Hybrid Monte Carlo study of monolayer graphene with …...PHYSICAL REVIEW B 96, 195408 (2017) Hybrid Monte Carlo study of monolayer graphene with partially screened Coulomb interactions
Author
others
View
0
Download
0
Embed Size (px)
344 x 292
429 x 357
514 x 422
599 x 487
Text of Hybrid Monte Carlo study of monolayer graphene with …...PHYSICAL REVIEW B 96, 195408 (2017) Hybrid...
PHYSICAL REVIEW B 96, 195408 (2017)
Hybrid Monte Carlo study of monolayer graphene with partially
screened Coulomb interactions at finite spin density
Michael Körner,1 Dominik Smith,1 Pavel Buividovich,2 Maksim
Ulybyshev,2 and Lorenz von Smekal1 1Institut für Theoretische
Physik, Justus-Liebig-Universität, 35392 Giessen, Germany
2Institut für Theoretische Physik, Universität Regensburg, 93053
Regensburg, Germany (Received 13 April 2017; revised manuscript
received 8 September 2017; published 6 November 2017)
We report on Hybrid Monte Carlo simulations at finite spin density
of the π -band electrons in monolayer graphene with realistic
interelectron interactions. Unlike simulations at finite
charge-carrier density, these are not affected by a fermion-sign
problem. Our results are in qualitative agreement with an
interaction-induced warping of the Fermi contours and a reduction
of the bandwidth as observed in angle-resolved photoemission
spectroscopy experiments on charge-doped graphene systems.
Furthermore, we find evidence that the neck-disrupting Lifshitz
transition, which occurs when the Fermi level traverses the van
Hove singularity (VHS), becomes a true quantum phase transition due
to interactions. This is in line with an instability of the VHS
toward the formation of ordered electronic phases, which has been
predicted by a variety of different theoretical approaches.
DOI: 10.1103/PhysRevB.96.195408
I. INTRODUCTION
Already the nearest-neighbor hexagonal tight-binding model [1]
qualitatively captures many of the interesting features of
monolayer graphene, such as the existence of massless electronic
excitations near the corners of the first Brillouin zone (K points)
with a linear dispersion relation for the low-energy excitations
around those Dirac points [2]. In the electronic bands, one also
finds saddle points, located at the M points, which are
characterized by a vanishing group velocity. These separate the
low-energy region, described by an effective Dirac theory, from a
region where electronic quasiparticles behave like a regular Fermi
liquid with a parabolic dispersion relation centered around the
points. See Fig. 1 for an illustration of the valence and
conduction bands of the nearest-neighbor tight-binding
theory.
When the Fermi level is shifted across the saddle points by a
chemical potential, a change of the topology of the Fermi surface
[which is one-dimensional for a two-dimensional (2D) crystal] takes
place. The distinct circular Fermi (isofrequency) lines surrounding
the Dirac points are deformed into triangles when the saddle point
is approached, meet to form one large connected region, and then
break up again into circles around the points (see Fig. 2). This is
known as the neck-disrupting Lifshitz transition [3].
The Lifshitz transition is not a true phase transition in the
thermodynamic sense (as it is purely topological and not associated
with any type of spontaneous symmetry breaking, i.e., formation of
an ordered phase), but exhibits features commonly associated with
such: singularities in free energy and susceptibility at zero
temperature with the chemical potential as the control parameter.
Unlike phase transitions, these singularities are logarithmic (in
two dimensions) and not due to interactions but to the vanishing
group velocity of electronic excitations at the saddle points,
which leads to a logarithmic divergence in the density of states
(DOS) with increasing surface area of the graphene sheet. This is
known as a van Hove singularity (VHS) [4] and can be observed in a
pure form, for instance, in microwave photonic crystals with a
Dirac spectrum as macroscopic models for the non-interacting
graphene band structure [5,6] and fullerenes with an Atiyah-Singer
index theorem [7].
The fate of the VHS of monolayer graphene in the presence of
many-body interactions is a topic of active research. Since
interactions are strongly enhanced by the divergent DOS, it is
generally believed that the VHS is unstable toward formation of
ordered electronic phases. This would imply that the Lifshitz
transition becomes a true phase transition in a realistic
description of the interacting system at sufficiently low
temperatures. It is known that superconductivity can arise from
purely repulsive interactions through the Kohn-Luttinger mechanism
[8]. Furthermore, it is known that VHSs exist close to the Fermi
level in most high-Tc superconducting cuprates, so it has long been
discussed whether they produce superconducting instabilities
generically (known as the “van Hove scenario” [9]). This scenario
was also proposed for doped graphene [10]. An exciting possibility
specific to graphene furthermore is the emergence of an anomalous
time-reversal symmetry violating chiral d-wave superconducting
phase from electron-electron repulsion close to the VHS
[11–17].
The theoretical perspective is not unambiguous, however. The
underlying reason is that several competing channels exist for
interaction-driven instabilities at the VHS, and that a subtle
interplay of different mechanisms (nesting of the Fermi surface and
deviations thereof, relative interaction strengths of couplings at
different distances, accounting for electron- phonon interactions,
etc.) can tilt the balance toward one phase or another. Aside from
d-wave superconductivity, different formalisms have, for example,
predicted superconductivity with pairing in a channel of f -wave
symmetry [18], spin- density wave (SDW) phases [19], a Pomeranchuk
instability [20,21], or a Kekulé superconducting pattern [22]. And
this is by no means an exhaustive list.
On the experimental side, by now there exist several techniques to
shift the Fermi level of graphene to the van Hove singularity: The
VHS can be probed in systems where gold nanoclusters are
intercalated between monolayer graphene and epitaxal graphene [23],
by chemical doping [10,24], by gating [25–27], or in “twisted
graphene” [28] (stacked graphene layers with a rotation angle).
Furthermore the valence and conduction bands of graphene can be
precisely mapped using angle-resolved photoemission spectroscopy
(ARPES). Such experiments show clear evidence for a reshaping of
the graphene bands by many-body interactions [29] and for
2469-9950/2017/96(19)/195408(17) 195408-1 ©2017 American Physical
Society
MICHAEL KÖRNER et al. PHYSICAL REVIEW B 96, 195408 (2017)
FIG. 1. Left: Electronic band structure of the nearest-neighbor
tight-binding theory of graphene. Dirac cones around the K points
are enlarged. Right: The first Brillouin zone and terminology for
special points therein.
a warping of the Fermi surface, leading to an extended, not
pointlike, van Hove singularity (EVHS) characterized by the
flatness of the bands, i.e., lack of energy dispersion, along one
direction [10].1 ARPES experiments on many different doped graphene
systems have also shown bandwidth renormalizations with deviations
of several hundred meV from single-particle band models [31] and a
massive enhancement of the electron-phonon coupling at the VHS
[24]. Unambiguously distinguishing different electronic phases
close to the VHS, however, is an open experimental challenge.
In this work, results of Hybrid Monte Carlo (HMC) simulations of
the interacting tight-binding theory of graphene are presented.
These simulations were carried out at finite chemical potential for
spin rather than charge density, as induced by a spin-staggered
chemical potential. Although the effects of the two are
substantially different, both kinds of chemical potential can be
used to tune Fermi levels across the entire range of the π bands,
including the VHS. The only difference, however substantial, is
that the spin-staggered chemical potential shifts the Fermi levels
of the two spin orientations in opposite directions corresponding
to the pure Zeeman splitting of an in-plane magnetic field
[32].
Technically this modification is necessary to avoid the
fermion-sign problem which otherwise arises from the com- plex
phase of the fermion determinant in the charge-doped system, and
which causes importance sampling to break down. The system with
spin-staggered chemical potential may be viewed as the so-called
“phase-quenched” version (defined by the modulus of the fermion
determinant in the measure) of graphene at finite charge density.
Because the two spin components of the π -band electrons in
graphene correspond to two different fermion flavors, this is
entirely analogous to simulating two-flavor QCD at finite isospin
density with pion condensation rather than finite baryon density in
the form of self-bound nuclear matter, which is equally impossible
due
1This is a rather general phenomenon which can also exist, e.g.,
around the saddle points in the dispersion relation of a triangular
lattice [30]. It is considered to be a crucial mechanism in the
context of the “van Hove scenario,” since it enhances the
singularity in the DOS and thus possible instabilities toward
ordered phases, such as superconductivity.
FIG. 2. Topology of the Fermi lines (intersection lines with
horizontal planes) for Fermi levels below (left), exactly at
(middle) and above (right) the saddle points.
to a strong sign problem. The phases are clearly distinct but many
important questions and genuine finite-density effects in lattice
simulations can be addressed at finite isospin density as
well.
The particular questions addressed here are about the genuine
effects of interelectron interactions on the VHS and the Lifshitz
transition in graphene. Our main focus is the behavior of
susceptibilities, which can be used to identify signatures of
instabilities and phase transitions. To directly study the
interaction-driven instabilities that might occur in the
charge-doped systems described above would require us to measure
the particle-hole susceptibility at finite charge density, which
is, however, not possible due to the sign problem. We therefore
simulate at finite spin density and measure the susceptibility
corresponding to ferromagnetic spin-density fluctuations instead,
which does not have this problem. In the noninteracting limit, the
two agree, and either one may be used to characterize the
electronic Lifshitz transition. Because the spin-staggered chemical
potential used here could at least in principle be realized in
experiment as well, by sufficiently strong in-plane magnetic
fields, our study might also become relevant in its own right in
the future.
We chose a realistic microscopic interelectron interaction
potential, which accounts for screening by electrons in the σ
bands [33]. A range of different system sizes and temperatures were
considered (these are temperatures of the electron gas only, as our
simulations presently do not account for phonons). Furthermore, the
interelectron interaction potential was rescaled to different
magnitudes, ranging from zero to the full interaction strength of
suspended graphene.
The purpose of this work is twofold: First, we wish to assess
whether the effects of interactions on the VHS at finite spin
density can at least qualitatively be compared with the
observations from ARPES data at finite charge density. To this end,
we study the reshaping of the π bands of the interacting system
(with respect to a “flattening” scenario). Second, we want to
exemplify how the logarithmic divergence of a susceptibility at the
VHS in the T → 0 limit can change to a critical scaling law at
nonzero Tc in the presence of interelectron interactions, as this
would signal the existence of
195408-2
HYBRID MONTE CARLO STUDY OF MONOLAYER . . . PHYSICAL REVIEW B 96,
195408 (2017)
an ordered electronic state close to the VHS and indicate that the
Lifshitz transition becomes a true quantum phase transition (with μ
as a control parameter) below this Tc. Identifying the precise
nature of the ordered phase, of course, will depend on the choice
of chemical potential and is thus beyond the scope of this
work.
This paper is structured as follows: In the following chapter, we
discuss the behavior of the particle-hole susceptibility in the
noninteracting tight-binding theory with temperature and system
size, where it agrees with that of the ferromagnetic spin-density
fluctuations. Exact results for the noninteracting system will
serve as a baseline for our studies of the effects of interelectron
interactions. As the HMC method necessitates the introduction of a
nonzero temperature of the electron gas (due to the introduction of
a Euclidean time dimension which must be of finite extent) and of
finite system size, the derivation accounts for both. Furthermore,
we derive the leading temperature dependence at the VHS, of the
divergent peak height of the susceptibility, in the infinite volume
limit. In Sec. III A the Hybrid Monte Carlo simulation of the
interacting theory is introduced, with emphasis on the fermion-sign
problem, which arises at finite chemical potential for charge-
carrier density. We derive expressions for the ferromagnetic and
antiferromagnetic spin-density susceptibilities expressed in terms
of the inverse fermion matrix. In Sec. IV, results of the HMC
calculations are presented. These include detailed studies of the
temperature- and interaction-dependent behavior of the
ferromagnetic susceptibility with particular emphasis on the fate
of the VHS. Preliminary results concerning the possibility of
spin-density wave order from the corresponding antiferromagnetic
susceptibility are also presented. We then provide our summary and
conclusions in Sec. V.
II. PARTICLE-HOLE SUSCEPTIBILITY AND LIFSHITZ TRANSITION
A. Noninteracting tight-binding theory
As mentioned in the introduction, in the nearest-neighbor
tight-binding description of the π bands in graphene, due to
particle-hole symmetry the particle-hole susceptibility is
independent of the sign of the chemical potential μ. Because this
is true independently for both spin components, there is thus no
distinction between the susceptibilities for charge and spin
fluctuations in the noninteracting case, and both equally reflect
the Lifshitz transition at finite charge or spin density. The
chemical potential μ this section can therefore be used for either
one interchangeably.
In order to understand the relation between the VHS in the
electronic quasiparticle DOS ρ(ω), the Thomas-Fermi susceptibility
χ and the properties of the neck-disrupting electronic Lifshitz
transition, one best starts from the particle- hole polarization
function (ω, p; μ,T ) at temperature T and chemical potential μ for
charge-carrier density (with μ = 0 at half filling), excitation
frequency ω, and momentum p.
The particle-hole polarization function determines the
charge-density correlations corresponding to the diagonal time
component of the polarization tensor in QED. Using the
imaginary-time formalism and subsequent analytic continu- ation
with the appropriate boundary conditions for retarded
Green’s functions, at one loop one arrives at the expression
(ω, p; μ,T )
]
×nf [β(s ′εk+ p − μ)] − nf [β(sεk − μ)]
s ′εk+ p − sεk − ω − iε , (1)
where gσ = 2 here for the spin degeneracy, φk = ∑ n eikδn
is the structure factor with nearest-neighbor vectors δn, n = 1,2,3
on the hexagonal lattice, and single-particle energies εk = κ|φk|
(where κ is the hopping parameter) in Fermi-Dirac distributions nf
(x) = 1/(ex + 1) at β = 1/T .
The particle-hole polarization or Lindhard function is a sum of
terms describing particle-hole excitations within the same band for
s ′ = s (intraband) and terms describing interband excitations for
s ′ = −s. The complete one-loop expressions for intraband and
interband transitions have been computed from Eq. (1) in closed
analytic form in Refs. [5,34].
The imaginary parts of vanish in the limit ω → 0 which describes
static Lindhard screening. In a subsequent long- wavelength limit p
→ 0, to which only interband excitations contribute, one obtains
the usual Thomas-Fermi susceptibility,
χ (μ) = Ac lim p→0
lim ω→0
here normalized per unit cell of area Ac = 3 √
3a2/2 with nearest-neighbor distance a ≈ 1.42 A for the carbon
atoms in graphene. It is straightforwardly calculated as
χ (μ) = gσAc
2T
)] . (3)
With the present normalization, the zero-temperature limit of χ (μ)
then in turn agrees with the density of states per unit cell ρ(ε)
at the Fermi level ε = μ, i.e.,
lim T →0
χ (μ) = gσAc
(2π )2 δ(εk − |μ|) ≡ ρ(μ). (4)
Figure 3 demonstrates explicitly how the integrand in Eq. (3)
encodes the effect of temperature on the susceptibility. The sharp
Fermi lines which were shown in the lower row of Fig. 2 are smeared
out, since a spread of different energy levels may now be excited.
The allowed range becomes narrower as temperature is lowered and
concentrates on the Fermi level with χ approaching the DOS there,
for T → 0, cf. Eq. (4).
The density of states was first derived for transverse vibrations
of a hexagonal lattice by Hobson and Nierenberg in 1953 [35]. They
found logarithmic divergences near the saddles of the energy bands,
i.e., the van Hove singularities, as well as the zeros now
identified with the Dirac points. From the corresponding analytical
expression of the hexagonal tight-binding model given in Ref. [36],
one readily obtains for the fermionic system at finite
charge-carrier density, with a Fermi energy near one of the van
Hove singularities
195408-3
MICHAEL KÖRNER et al. PHYSICAL REVIEW B 96, 195408 (2017)
FIG. 3. Integrand of Eq. (3) for values of μ below (right), at
(middle), and above (left) the van Hove singularity; from the top
to the bottom row the temperature has been lowered by a factor 1/2
(from T = κ/2 to κ/4).
at μ = ±κ ,
κ −1
(5)
The correspondingly diverging zero-temperature susceptibility χ is
due to the infinite degeneracy of ground states of the two-
dimensional fermionic system when the Fermi level passes through
the van Hove singularity. In the thermodynamic sense, this can be
considered as a zero-temperature transition with control parameter
|μ|. To illustrate, this one introduces the re- duced Fermi-energy
parameter z = (|μ| − κ)/κ to rewrite (5)
χ (z) = 3gσ
2π2κ [− ln |z| + 2 ln 2 + O(z)]. (6)
Unlike the cases of first- or second-order phase transitions, the
susceptibility does not diverge with a power law but
logarithmically. This is a manifestation of the neck-disrupting
electronic Lifshitz transition in two dimensions [3,37]. There is
no obvious change in symmetry; the transition is only due to the
topology change of the Fermi surface. The singular part of the
corresponding thermodynamic grand potential is nonzero on both
sides of the transition. The original argument is simple: One
expands the single-particle energy around a saddle point at κ in
suitable coordinates,
εk = κ + k2 x
2m1 − k2
ρs(z) = −gσAc
For the nearest-neighbor tight-binding model on the hexagonal
lattice, one verifies that
√ m1m2 = 1/(κAc) so that ρs(z) =
−gσ /(2π2κ) ln |z|. With a factor of 3 for the three M points per
Brillouin zone, this agrees with the leading behavior of the
zero-temperature susceptibility in Eq. (6), as it should. One
integration over κz then yields the number of states in an interval
around the saddle, a second one the corresponding
contribution to the grand potential per unit cell which hence
acquires a corresponding singularity [37]
sing = 3gσ κ
2 ln |z|. (9)
It is symmetric around z = 0. There is thus no order parameter in
the usual sense, but one may discuss this transition in terms of a
change in the approximate symmetries of the low- energy excitation
spectrum with some analogy in excited-state quantum phase
transitions [5].
At any rate, the logarithmic singularity of the electronic Lifshitz
transition in the grand potential is restricted to strictly zero
temperature. To see this explicitly, we first use the density of
states to express the finite-temperature susceptibility in the
following form:
χ (μ) = 1
2T
)] . (10)
Assuming μ > 0 for now, we may drop the second term in the
brackets for sufficiently low temperatures and extend the limits of
integration to ±∞. For the susceptibility maximum at μ = κ , we can
furthermore approximate ρ(ε) by the expansion in Eq. (5) in the
region of support of the integrand around ε = κ to obtain
χmax = 3gσ
2π2κ {− ln (πT /κ) + γE + 3 ln 2 + O(T )}, (11)
where γE is the Euler-Mascheroni constant. The maximum of the
susceptibility of the electronic Lifshitz transition is finite at
finite T .
In this way, the logarithmic divergence in the DOS at the VHS is
reflected in the Thomas-Fermi susceptibility χ (μ). At low but
finite temperatures, χ (μ) peaks when the Fermi level crosses the
VHS (for μ = κ in the noninteracting system). The peak height grows
logarithmically as temperature is lowered. Its divergence in the
zero-temperature limit is a manifestation of the neck-disrupting
electronic Lifshitz transition with its logarithmic singularity in
the chemical potential as the corresponding control
parameter.
So much for the noninteracting and infinite system. Before we
discuss finite volume effects and interactions, we can speculate
how a reshaping of the saddle points in the single- particle band
structure by interactions might qualitatively affect the Lifshitz
transition. If we assume a non-Fermi liquid behavior near the
saddles, for example, of the form
εk = ε0 + κ[c1(kxa)α − c2(kya)α], (12)
instead of (7), where we had √
c1c2 = 3 √
3/4, ε0 = κ, and α = 2 for the noninteracting tight-binding model,
we now obtain analogously
ρs(z) ∝ κ−1|z|−γ , with γ = 1 − 2
α . (13)
In Eq. (10), this for μ = ε0 then readily yields
χmax ∝ 1
κ
( κ
T
)γ
, (14)
195408-4
HYBRID MONTE CARLO STUDY OF MONOLAYER . . . PHYSICAL REVIEW B 96,
195408 (2017)
replacing Eq. (11) for γ = 0. We can see that, e.g., for α = 4 in
single-particle energies near the saddles (12), the logarithmic
divergence of Eq. (11) turns into a square root divergence of the
susceptibility maximum for T → 0 with γ = 1/2, whereas the limit of
a completely flat single-particle energy band with α → ∞ would
correspond to γ = 1 and hence χmax ∝ 1/T .
We conclude this section by reiterating that for vanishing two-body
interactions, χ (μ) is blind to a change of sign. And this is true
for each of the spin orientations separately. We will use opposite
signs of μ for the two spin orientations in our simulations below
to avoid a fermion-sign problem. While this then corresponds to a
Zeeman splitting, as caused by an in-plane magnetic field, for
example, rather than a change of the charge-carrier density away
from half filling, the tight- binding results are unaffected by
such a sign change. We may therefore thus use χ (μ) with
unlike-sign chemical potentials for the two spin states, analogous
to isospin chemical potential in quantum chromodynamics (QCD), to
detect deviations from the pure tight-binding theory in our Hybrid
Monte Carlo (HMC) simulations, where it can be readily obtained
(discussed in Sec. III C).
To make the comparison between the Lifshitz transition in the
noninteracting system and the results from HMC simulations with
interactions as direct as possible, in the next subsection we first
derive semianalytic expression for χ (μ) in the tight-binding model
on finite lattices with the same boundary conditions that we use in
the simulations.
B. Finite lattices
In our HMC simulations, we study graphene sheets of finite surface
area, with periodic boundary conditions along the primitive vectors
a1,2 = a
2 ( √
3, ± 3) (where a ≈ 1.42 A is the interatomic distance on the
hexagonal lattice) spanning one of the triangular sublattices
(“Born-von Kármán boundary conditions”). We simulate symmetric
lattices, with N unit cells along each axis. To take finite size
into account, Eq. (3) is rewritten as a sum over the allowed
momentum states, which are given by the Laue condition eik R = 1,
where R = na1 + ma2 with n,m ∈ [1, . . . ,N]. The momentum states
are
k = n
( √
3,±1) are the the base vectors of the recip- rocal lattice. The
integral measure d2k turns into a finite surface element (k)2 = |b1
× b2|/N2 = ABZ/N2, where ABZ = (2π )2/Ac is the area of the first
Brillouin zone, and the integral in Eq. (3) for the susceptibility
of a finite sheet becomes
χ (μ) = gσ
(16)
Here εmn is the dispersion relation, evaluated at the points
defined by Eq. (15):
εmn = κ
0.2
0.4
0.6
0.8
1.0
N
−1
FIG. 4. Finite-size scaling of the susceptibility peak at different
temperatures (β = 1/T ) from Eq. (16); the horizontal lines
indicate the leading-order prediction from Eq. (11) and the slight
deviations of the infinite volume limit from this prediction for β
= 2 eV−1 are due to O(T ) corrections.
Equation (16) is of a form which can be compared directly to the
simulations. The sums cannot be carried out analytically, but are
straightforward to evaluate numerically.
Of course, there is no divergence of the particle-hole
susceptibility in a finite volume, not even at zero temperature.
The spectrum is discrete and the total number of states is finite,
so the density of states cannot diverge either. In Ref. [5] it was
shown, however, that the finite-size scaling of the susceptibility
maximum at T = 0 is logarithmic likewise, namely
χmax = 3gσ
2π2κ [ln Nc − 2 ln π + 1 + O(1/Nc)], (18)
where Nc = N2 is the number of unit cells. Since our simulations
are carried out at finite temperature, it is clear that we cannot
observe this behavior directly because it is valid only at strictly
zero temperature. The extension of the analytic expressions to
finite volume and finite temperature is not so straightforward,
however, and cannot be done analytically.
Therefore, we use the implicit representation of χ (μ) for a finite
sheet at temperature T in Eq. (16) and compute the sums
numerically. The results of χ at μ = κ are shown for various
lattice sizes and temperatures in Fig. 4. In general, for any
finite temperature, χ (μ = κ,N ) for N → ∞ approaches a flat
asymptote ∝ ln(βκ), which in turn increases with β = 1/T
according to Eq. (11). It is the temperature dependence of these
asymptotic values which follows Eq. (11). Convergence to the
infinite volume limit becomes slower for decreasing temperatures as
the asymptotic value increases.
Figure 4 shows a strong influence of the parity of the lattice,
where odd lattices approach the N → ∞ limit from below and even
lattices from above. For a fixed lattice size, the peak height
either diverges (for even lattices) or goes to zero (for odd
lattices) as T → 0. This difference arises from the fact that the
sums in Eq. (16) only contain momentum modes which hit the M points
exactly when N is even. For even N , points on the lines with
sech2((εmn − μ)/2T ) = 1 contribute with diverging weight ∝1/T to
the sum (cf. Fig. 3), while for odd
195408-5
MICHAEL KÖRNER et al. PHYSICAL REVIEW B 96, 195408 (2017)
N there are no such points but only points that cluster around
these lines when the system becomes large.
III. INTERELECTRON INTERACTIONS
A. Simulation setup
The present work implements Hybrid Monte Carlo simula- tions of the
interacting tight-binding theory on the hexagonal graphene lattice,
based on a formalism developed by Brower et al. [38,39], which goes
beyond the low-energy approxi- mation (studied extensively in the
past [40–49]) and is thus able to capture the full band structure
beyond the Dirac cones. The HMC method on the graphene lattice is
by now well established, and has been successfully applied in
conclusive studies of the antiferromagnetic phase transition
[50–54] as well as in ongoing studies of the phase diagram of an
extended fermionic Hubbard model on the hexagonal graphene lattice
[55]. Numerous other topics were also addressed with HMC, such as
the optical conductivity of graphene [56], the effect of hydrogen
adatoms [57,58], and the single quasiparticle spectrum of carbon
nanotubes [59].
We have written about our setup in great detail in the past (see
Ref. [53] for a step-by-step derivation) and will only provide a
summary here. In particular, we focus on the additional challenges
which arise when introducing a chemical potential (i.e., the
fermion-sign problem) and discuss our work-around solution (a
spin-dependent sign flip). To be clear, this work does not attempt
to solve the sign problem but rather studies a modified Hamiltonian
which is free of such a problem. Assessing to what degree the
physics is changed by this modification is part of the motivation
for this work.
The starting point is the interacting tight-binding Hamilto- nian
in second-quantized form
H = ∑ x,y
+ ∑ x,y
qxVxyqy + ∑
x
ms(a † xax + b†xbx). (19)
The chemical potential is absent at this stage and will be
introduced later. The first sum in Eq. (19) runs over pairs of
nearest neighbors only (with a hopping parameter κ = 2.7 eV), so we
neglect higher order hoppings. The other sums run over all sites
(including both sublattices) of the 2D hexagonal lattice. Here
a
† x,ax denote creation and annihilation operators
for electrons in the π bands with spin +1/2 in the z direction
(perpendicular to the graphene sheet) and b
† x,bx are analogous
operators for holes (antiparticles) with spin −1/2. The hopping
term also contains a sublattice dependent sign flip for the b
† x,bx
operators [53]. We have also added in Eq. (19) a staggered mass
term
ms = (−1)s m with a sublattice s = 0,1 dependent sign to regulate
the low-lying eigenvalues of the Hamiltonian, as is customary in
lattice-QCD simulations. While simulations at exactly zero mass are
possible in principle [55] (unlike lattice QCD, there appear to be
no topological obstructions to simulating at exactly zero mass
here), a finite mass term has numerical advantages, and it only
affects the low-lying excitations around the Dirac points, which
are not the primary
focus of our present study. In fact, our investigation of the
Lifshitz transition turns out to be rather insensitive to this mass
term as one might expect, based on the band structure of the
noninteracting system, as long as ms κ . Moreover, a spin- and
sublattice-staggered mass term of this form also serves as an
external field for sublattice symmetry breaking by spin-density
wave formation, so derivatives with respect to ms
may be used to detect an instability of the ground state toward SDW
order.
The operator qx = a † xax − b
† xbx represents physical charge.
Interactions are taken to be instantaneous, which is true to good
approximation since vF c, where vF is the Fermi velocity of the
electrons. One of the great advantages of the instantaneous
Hamiltonian in Eq. (19) (compared to implementing the photon as an
Abelian gauge field on link variables) is that any
positive-definite matrix can be chosen for Vxy , leaving great
freedom to choose a realistic two-body potential to describe
microscopic interactions. In particular, it is possible to
implement deviations from pure Coulomb-type interactions due to
screening from σ band and other localized electrons.
In this work, we choose a two-body potential, which accounts for
precisely this screening as obtained from cal- culations within a
constrained random-phase approximation (cRPA) by Wehling et al. in
Ref. [33]. Therein exact values were obtained for the onsite U00,
nearest-neighbor U01, next-nearest-neighbor U02, and
third-nearest-neighbor U03 interaction parameters, and a
momentum-dependent phe- nomenological dielectric screening formula
derived, based on a thin-film model, which can be used to
interpolate to an unscreened Coulomb tail at long distances. Here
we use the “partially screened Coulomb potential” of Ref. [53],
which combines both results via a parametrization based on a
distance-dependent Debye mass mD . The matrix elements Vxy
are then filled using
(20)
where a is the nearest-neighbor distance as before, and mD , m0, c,
and γ are piecewise constant chosen such that mD,m0 →0 and c,γ → 1
for r a. For the precise values of these parameters, we refer to
the tables in Ref. [53]. The resulting interaction potential is
shown in comparison to the unscreened Coulomb potential in Fig.
5.
We note in passing that there is still some theoretical uncertainty
concerning the screening effects generated by the σ -band electrons
at short distances (for a detailed discussion, see Ref. [60]). For
the purpose of our present study, this is of minor importance
because our main conclusions should be insensitive to small
variations of the short-range interaction parameters. Larger
variations of these parameters, on the other hand, can lead to very
rich phase diagrams including topologi- cal insulating phases [61].
A detailed study of competing order from HMC simulations of the
extended Hubbard model on the hexagonal lattice with varying
on-site and nearest-neighbor couplings is currently in progress
[55].
To proceed, one derives a functional-integral formulation of the
grand-canonical partition function Z = Tr e−βH , in which the
ladder operators are replaced by Grassman valued fermionic field
variables, by factorizing e−βH into Nt terms
195408-6
HYBRID MONTE CARLO STUDY OF MONOLAYER . . . PHYSICAL REVIEW B 96,
195408 (2017)
standard Coulomb potential
2
4
6
8
10
r/a
) in
eV
FIG. 5. Comparison of the standard Coulomb potential (red) with the
partially screened potential given by Eq. (20). The first four
points are exact cRPA results of Ref. [33] (green), while the
remaining ones are obtained from the interpolation based on the
thin-film model from the same reference (blue).
(taken to be “slices” in Euclidean time) and inserting complete
sets of fermionic coherent states. Formally, Nt must be taken to
infinity to obtain an exact result, but for numerical simulations
Nt is a finite number. This implies a discretization error of order
O(δ2), where δ = β/Nt . The final result is
Z = ∫ Nt−1∏
x,t+1ηy,t )
x,t+1(ηx,t+1 − ηx,t )]
Here we have used the notation Qx,t,t ′ = ψ∗ x,tψx,t ′ − η∗
x,tηx,t ′ . We would now like to integrate out the fermionic
fields
to obtain an expression containing only determinants of a fermionic
matrix M , which can then be sampled stochastically. This is
prevented by fourth powers of the fields, appearing in the
interaction term ∼qxVxyqy . These can be removed by a
Hubbard-Stratonovich transformation
exp
{ − δ
2
∑ x,y
qxVxyqy
∑ x
φxqx
} , (22)
at the expense of introducing an additional dynamical scalar field
φ (“Hubbard field”). The resulting expression contains only
quadratic powers, so Gaussian integration can be carried out, which
yields
Z = ∫ [∏
x,t
φx,t
} , (23)
A subtlety here is that, if the Hubbard-Stratonovich trans-
formation (22) is naively applied to Eq. (21), the determinant of
the fermion matrix is a high-degree polynomial of the noncompact
field φ whose numerical evaluation is plagued by uncontrollable
rounding errors. It is therefore advantageous to use an alternative
fermion discretization with a coupling to a compact Hubbard field
[38,51,53]. Its derivation is slightly more involved but
straightforward, essentially based on applying the
Hubbard-Stratonovich transformation before introducing the
fermionic coherent states. The matrix elements are then computed
using the identity
ξ | e ∑
[∑ x,y
′ y
] , (24)
which holds for arbitrary matrices A. Here, A is a diagonal matrix
with elements Axx = ±iδ φx . The differences are of subleading
order δ2 in the time discretization. Hence, both are equivalent at
the order δ and share the same continuum limit. It is this modified
version of the fermion matrix M(φ), with the compact Hubbard field,
which is used for numerically stablility in our simulations. Its
matrix elements are given by (for details, see Ref. [53])
M(x,t)(y,t ′)(φ) = δxy
β
Nt
(25)
The matrix contains terms corresponding to the different con-
tributions from the tight-binding Hamiltonian and a covariant
derivative in Euclidean time, in which the Hubbard field enters in
form of a gauge connection where φ acts as an electrostatic
potential.
Both M and M† appear in Eq. (23) due to the two spin orientations
entering as independent degrees of freedom into the Hamiltonian (we
are essentially treating spin-up and spin-down states as different
particle flavors). The resulting expression is suitable for
simulation via HMC at half filling (μ = 0), as the integrand may be
interpreted as a weight function for the Hubbard field φ.
B. Hybrid Monte Carlo and the fermion-sign problem
The HMC method (originally developed for strongly interacting
fermionic quantum field theories [62]) consists in essence of
creating a distribution of field configurations representative of
the thermal equilibrium, by evolving the φ field in computer time τ
through a fictitious deterministic
195408-7
MICHAEL KÖRNER et al. PHYSICAL REVIEW B 96, 195408 (2017)
dynamical process, governed by a conserved classical Hamil- tonian
defined in the higher dimensional space spanned by real Euclidean
spacetime and τ . Quantum fluctuations enter in the form of
stochastic refreshments of the canonical momentum π
associated with the Hubbard field φ. As a symplectic integrator
must be used to solve Hamilton’s equations for φ and π , an
additional error arises from the finite step size of this
integrator, which is subsequently corrected by a Metropolis
accept-reject step. HMC is thus an exact algorithm (see Ref. [53]
for further details).
HMC is a form of importance sampling, i.e., a method of
approximating the functional integral by probabilistically
generating points in configuration space which are clustered in the
regions that contribute most to the integral. A crucial criterion
for its applicability is the existence of a real and
positive-definite measure for the dynamical fields, which may then
be interpreted as a probability density. This is true here only
because the phases of M and M† cancel exactly in Eq. (23). As we
will see, this no longer holds at nonzero charge density.
To generate finite charge-carrier density, one would have to add a
corresponding chemical potential μ, replacing the Hamiltonian in
Eq. (19) by
H → H − μ ∑
(a† xax − b†xbx). (26)
At the level of the partition function, this leads to the
modification
Z(μ) = ∫ Nt−1∏
(27)
After integrating out the fermion fields, one obtains a modified
version of Eq. (23),
Z = ∫ [∏
x,t
φx,t
Nt
= M†(φ,−μ)(x,t)(y,t ′). (29)
There is no cancellation of phases in Eq. (28); thus importance
sampling breaks down, as we no longer can interpret the integrand
as the weight of a given microstate in the ensemble. This is at the
root of the fermion-sign problem. Whether it is a hard problem or
not depends on the expectation value of
FIG. 6. Histograms of the phase of det M(φ,μ)/ det M(φ,−μ) obtained
from a 6 × 6 lattice at β = 2 eV−1 for different μ, at 10% of the
interaction strength of suspended graphene. The results are modeled
with Gaussian (μ = 0.15 and 0.30 eV−1) and uniform (μ = 0.45 eV−1)
distributions respectively. The inlay shows the adjusted R2 for
fitting a constant to the data at a range of different μ. For μ 0.4
eV the numerical data are well described by a uniform distribution,
indicating a hard sign problem.
the phase of the determinant in the “phase-quenched” theory defined
by the modulus of the fermion determinant in the measure; i.e.,
writing
Z = ∫ [∏
x,t
φx,t
det M(φ,−μ)
} , (30)
we consider the complex ratio of determinants with opposite- sign
chemical potentials as an observable in the phase- quenched theory
with partition function Zpq and
Z(μ)
Zpq(μ) =
⟩ pq
. (31)
Obviously this ratio is unity at half filling (i.e., for μ → 0) and
at vanishing interaction strength for all μ, because the
noninteracting tight-binding theory is blind to the sign of μ
for each spin component individually. To exemplify that the signal
is indeed lost quickly, however,
when the chemical potential for charge-carrier density is tuned
away from half filling in the interacting theory, we have measured
the modulus and the complex phase of the ratio of determinants in
Eq. (31) on a 6 × 6 lattice, at β = 2 eV−1
and 10% of the interaction strength of suspended graphene. This
method of “reweighting” therefore certainly fails near the van Hove
singularity, already at rather moderate interaction strengths.
Figure 6 shows histograms of the phase for different values of μ
together with fit-model curves. As a measure for the
signal-to-noise ratio we have used the adjusted R2
associated with attempting to model the histograms with a
195408-8
HYBRID MONTE CARLO STUDY OF MONOLAYER . . . PHYSICAL REVIEW B 96,
195408 (2017)
uniform distribution (this quantity is 0 for a strictly nonlinear
relation between the data and the fitted curve and 1 for a perfect
linear dependence). As one can see in the figure, the adjusted R2
of the constant fit shows a rather rapid crossover and approaches
values close to 1 at μ ≈ 0.4 eV, which indicates that the signal is
lost in the noise already on the 6 × 6 lattice. The effect will be
further enhanced with increasing lattice sizes. Note that the
modulus of the ratio of determinants is not unity here either. In
fact, it also decreases with μ. As usual, however, it is the phase
fluctuations that are primarily responsible for the loss of signal
due to cancellations.
The underlying physical reason for a nonpolynomially hard
signal-to-noise-ratio problem typically is that the overlap of
phase-quenched and full ensembles tends to zero exponentially
because of a complete decoupling of the corresponding Hilbert
spaces in the infinite-volume limit when the two ensembles
correspond to excitations above different finite-density ground
states (here charge-carrier versus spin density). An exponential
error reduction might be possible with generalized density-of-
states methods [63], which work beautifully in spin systems [64]
and heavy-dense QCD [65] but have yet to be applied to strongly
interacting theories with dynamical fermions.
Dense fermionic theories with a sign problem are a very active
field of research and we cannot cover the vast body of literature
here. There is no general solution, however.
Sometimes cluster algorithms [66] or extensions thereof that
exploit cancellations of field configurations [67] help. On the
other hand, when they do, there also appears to be an underlying
Majorana positivity [68–70] and the theory therefore really is free
of a sign problem as in the case of the antiunitary symmetries,
such as time-reversal invariance with Kramers degeneracy discussed
below.
Sometimes it is possible to simulate dual theories with worm
algorithms [71,72]. Deformation of the originally real
configuration space into a complex domain can help by either
sampling Lefschetz thimbles of constant phase [73], reducing the
sign problem to that of the residual phases, or more generally,
field manifolds with a milder sign problem obtained from
holomorphic gradient flow [74]. Doubling the number of degrees of
freedom by complexification one can also try a complex version of
stochastic quantization, i.e., by simulating the corresponding
complex Langevin process [75].
While all these techniques have their difficulties and are actively
being further developed, in the meantime we follow a different
strategy here. This is to simulate a sign-problem-free variant of
the original theory with standard Monte Carlo techniques and study
genuine finite-density effects where importance sampling is
possible. Such variants could be theories with antiunitary
symmetries such as two-color QCD, with two instead of the usual
three colors [76,77], or G2 QCD, with the exceptional Lie group G2
replacing the SU(3) gauge group of QCD [78,79].
The arguably simplest variant is the phase-quenched theory itself,
however. In two-flavor QCD, this amounts to simulating at finite
isospin density [80,81]. Here it corresponds to introducing a
chemical potential for finite spin density, like a pure Zeeman term
from an in-plane magnetic field, rather than one for finite
charge-carrier density, as mentioned above. To this end, we add a
chemical potential μσ = (−1)σμ with a spin σ = 0,1 (for up or down)
dependent sign; i.e., instead of
(26) we use the replacement
H → H − μ ∑
(a† xax + b†xbx). (32)
Compared to (26), the sign of the term ∼b † xbx has been
flipped.
This leads to a modification of the spin-down determinant in Eq.
(29), such that
M(φ,μσ )(x,t)(y,t ′) = M†(φ,0)(x,t)(y,t ′) − μ β
Nt
= M†(φ,μ)(x,t)(y,t ′). (33)
Cancellation of the phases in the partition function is thus
restored; μσ shifts the Fermi surfaces for electronlike and
holelike excitations in opposite directions. As the nearest-
neighbor tight-banding bands are symmetric under exchange of
particlelike and holelike states individually for each spin, the
Lifshitz transition in the noninteracting theory is in fact blind
to this change of sign. As a result, μσ induces a Zeeman splitting
but without the phase factors from a Peierls substitution in the
hopping term. It therefore describes graphene coupled to an
in-plane magnetic field [32]. In the following, we will omit the
spin index. It is implied that μ is spin staggered from now on,
i.e., corresponding to μσ = (−1)σμ as in Eq. (32).
C. Observables
Expectation values of physical operators in the thermal ensemble
are expressed in the path-integral formalism as
O = 1
∫ Dφ O(φ) det(MM†)e−S(φ). (34)
Their representation in the space of field variables can be
obtained from derivatives of the partition function with respect to
corresponding source terms. We are interested in the particle-hole
susceptibility (2), which up to a factor of β = 1/T agrees with the
number susceptibility (per unit cell).2
Hence, it is given by
χ (μ) = − 1
)2 ] , (35)
where = −T ln Z is the grand-canonical potential and Nc = N2 is the
number of unit cells. Using the path-integral representation of Z,
we can express χ (μ) in terms of the fermion matrix M(φ),
since
1
Z
dnZ
d
( M−1 dM
dμ
) (37)
2Of course, with the spin-staggered μ it is strictly speaking not a
number but a spin, i.e., magnetic susceptibility; see above.
195408-9
MICHAEL KÖRNER et al. PHYSICAL REVIEW B 96, 195408 (2017)
and
d2
χcon(μ) = −2
)⟩2} , (39)
where χcon/dis denote the connected and disconnected contri-
butions respectively. The brackets on the right-hand sides of Eqs.
(39) are understood as averages over a representative set of field
configurations. The traces can be evaluated with noisy
estimators.
A susceptibility χ sdw corresponding to the fluctuations of the
antiferromagnetic spin-density wave order parameter computed at
half filling in Ref. [55] can be obtained in complete analogy to
the above, replacing all derivatives with respect to μ by
derivatives with respect to the sublattice- staggered mass ms =
(−1)s m in Eq. (19). The resulting expressions are then of
precisely the same form as Eqs. (39), with the replacement μ →
m,
χ sdw con (μ) = −2
Ncβ
⟨ ReTr
Ncβ
{⟨[ ReTr
)⟩2} . (40)
IV. RESULTS
In this section, we first present our results for the suscepti-
bility χ (μ) of ferromagnetic spin-density fluctuations, i.e., the
spin-staggered particle-hole susceptibility, from Hybrid Monte
Carlo simulations of the interacting tight-binding theory at finite
spin density and temperature. Only in the last subsection do we
briefly come back to the spin-density dependence of the
antiferromagnetic SDW susceptibility χ sdw as well.
All results were obtained from hexagonal lattices of finite size
with periodic Born–von Kármán boundary conditions, with an equal
number of unit cells in each principal direction. We chose a
sublattice and spin-staggered mass ms of magni- tude m = 0.5 eV, an
interatomic spacing of a = 1.42 A, and a hopping parameter of κ =
2.7 eV. We furthermore use the partially screened Coulomb potential
discussed in data in Sec. III A and Ref. [53].
The rescaled effective interaction strength αeff is defined in the
following as αeff = λαgraphene with αgraphene = e2
hvF ≈ 2.2
(λ thus acts as a global rescaling factor which changes each
element of the interaction matrix in the same way, i.e., Vxy →
λVxy). Interactions were rescaled to different magnitudes in the
range λ = [0,1] (spanning the range from no interactions to
suspended graphene, i.e., without any substrate-induced dielectric
screening).
For each set of parameters presented in the following, measurements
were done in thermal equilibrium on at least 300 independent
configurations of the Hubbard field. Integrator step sizes were
tuned such that the Metropolis acceptance rate was always above
70%. All error bars were calculated taking possible
autocorrelations into account, using the binning method and
standard error propagation where appropriate. For calculation of
observables, all traces are estimated with 500 Gaussian noise
vectors.
A. Influence of the Euclidean-time discretization
As HMC simulations are carried out at finite discretization δ
of the Euclidean time axis (which is related to the temperature
through the relation β = δNt , where Nt is the number of time
slices), exact quantitative results can be only obtained by δ → 0
extrapolation. As it would be computationally prohibitively
expensive to simulate for a suitable range of δ values with each
set of physical parameters (in particular, when temperatures are
low, system sizes are large or interactions are strong), we carry
out such an extrapolation only for a few exemplary cases. This will
help to develop an understanding of the systematics of the
discretization errors in order to assess whether simulations with a
fixed discretization can provide reliable results at rea- sonable
cost, in particular for the low temperatures which are required to
detect deviations from the logarithmic divergence of χ (μ = κ).
Such is the purpose of this section.
Figure 7 (top) shows the trivial case of χ (μ) at vanishing
two-body interactions, corresponding to a Hubbard field φ
which is set to zero on all lattice sites. The inversions of the
fermion matrix in Eqs. (39) are straightforward to carry out in
this case and no molecular dynamics trajectories are in fact needed
at all. Furthermore, the disconnected part of χ (μ) vanishes
exactly in this case, as the expectation value ReTr (. . .)2
factorizes. The different curves represent calculations for
different values of δ, on an N = 12 lattice at β = 2 eV−1 (from
Fig. 4 we know that finite-size effects can be neglected for this
choice), together with a point-by-point δ → 0 extrapolation using
quadratic polynomials. As we expect, the extrapolated points agree
well with the semianalytic calculation from Eq. (16), with small
deviations only arising from the uncertainty associated with the
fitting procedure. We also see that the main effect of finite δ is
a shift to lower and in some areas negative values. Fortunately,
the shift is nearly constant over the entire range of μ. A similar
behavior can be seen when interactions are switched on. Figures 7
(middle and bottom) again show results from the N = 12 lattice at β
= 2 eV−1 (for Nt between 12 and 96) but with nonzero interaction
strengths corresponding to λ = 0.4 and λ = 1.0 respectively. For
comparison, as a first indication of the effects of interactions,
we also show the noninteracting limit in these figures. In order to
illustrate the origin of the discretization errors in the
interacting case, in Figs. 8 we also display χcon(μ) (top) and
χdis(μ) separately for λ = 1.0. What is striking is that the
disconnected part seems to depend only very weakly on
195408-10
HYBRID MONTE CARLO STUDY OF MONOLAYER . . . PHYSICAL REVIEW B 96,
195408 (2017)
FIG. 7. χ (μ) for λ = 0.0 (top), λ = 0.4 (middle), and λ = 1.0
(bottom) at β = 2 eV−1, N = 12. Different discretizations are shown
as well as pointwise quadratic δ → 0 extrapolations (blue). The
semianalytic λ = 0.0 result obtained from Eq. (16) is shown for
comparison in all plots (gray).
δ, while the connected part displays the familiar shift. This is a
fortunate situation, as it is χdis which is expected to show the
characteristic scaling indicative of a true thermodynamic phase
transition.
Our main conclusion here is that we have good justification to
assume that the effect of interactions can be studied qualitatively
rather well for fixed δ. Nevertheless, we present a set of fully
extrapolated results for β = 2 eV−1 in the following section.
Results for lower temperatures will then be presented for fixed
δ.
FIG. 8. χcon(μ) (top) and χdis(μ) (bottom) for λ = 1.0 at β = 2
eV−1, N = 12 for different discretizations (red) and their
pointwise quadratic δ → 0 extrapolations (blue).
B. Influence of inter-electron interactions
To demonstrate the effects of interelectron interactions, we have
carried out the same δ → 0 extrapolations for β = 2 eV−1, N = 12,
and λ ∈ {0.1,0.4,0.8,1.0}. As before, δ val- ues where chosen from
the set δ ∈ { 1
6 , 1 12 , 1
18 , 1 24 , 1
30 , 1 36 , 1
48 }eV−1
(corresponding to Nt ’s between 12 and 96), and second-order
polynomials were used in all cases (the full set of δ values was
only used for the cases λ = 0.8/1.0). In Figs. 9 we have collected
the extrapolated results for the various interaction strengths,
showing the full susceptibility (top) and the con- nected (middle)
and disconnected (bottom) parts respectively. We observe that with
increasing interaction strength the peak of the full susceptibility
at the VHS becomes more pronounced. This is due to both a
corresponding rise in the connected part at the VHS and an
additional contribution from the disconnected part (which is
clearly nonzero for the interacting system). The peak position as
well as the upper end of the conduction band are shifted toward
smaller values of μ. Note that we cannot disentangle the squeezing
of the π bandwidth from interactions and doping here. The combined
effect certainly increases with increasing interaction strength
which is qualitatively in line with experimental observations [31].
Additionally, we observe that the thermodynamically interesting
disconnected part χdis
of the susceptibility develops a second peak close to the upper end
of the band (corresponding to the point), which is thus a purely
interaction-driven effect.
195408-11
MICHAEL KÖRNER et al. PHYSICAL REVIEW B 96, 195408 (2017)
FIG. 9. χ (μ) (top), χcon(μ) (middle), and χdis(μ) (bottom) for β =
2 eV−1, N = 12 at different interaction strengths. All displayed
points are quadratic δ → 0 extrapolations from simulations at
nonzero δ.
From Figs. 9 (top and middle) it also appears that the con- nected
part χcon(μ) is slightly negative at large values of μ. This is
clearly unphysical. We attribute it to a residual systematic error
associated with the δ → 0 continuum extrapolations. We have checked
that with quadratic polynomial fits the negative offset shrinks as
additional points with smaller δ are included.
C. Influence of temperature
This section focuses on the effect of electronic temperature (as no
phonons are included, the temperature of the lattice atoms is zero
by definition). All results presented in the
FIG. 10. Temperature dependence of χ (μ) (top), χcon(μ) (mid- dle)
and χdis(μ) (bottom). Lattice sizes scale linearly with β, such
that the displayed curves correspond to N = 12,18,24 respectively;
with δ = 1/6 eV−1 and λ = 1 for all cases.
present section were obtained for λ = 1. Figures 10 show results
for χ (μ) (top), χcon(μ) (middle), and χdis(μ) (bottom)
respectively over the entire range of the conduction bands for
different temperatures. Proper lattice sizes for each temper- ature
were chosen such that finite-size effects play no role (we first
estimated the necessary lattice sizes from Fig. 4, and subsequently
verified the stability of the results under further increase of N
for individual points). All results were obtained with δ = 1/6
eV−1, which leads to a rather large negative shift of the entire
curves. Nevertheless, a clear signal can be seen for an increase of
χ (μ), not only at the VHS but at the upper end of the band as
well. What is even more striking is that from a
195408-12
HYBRID MONTE CARLO STUDY OF MONOLAYER . . . PHYSICAL REVIEW B 96,
195408 (2017)
(T)
con(T)
dis(T)
0.1
0.2
0.3
0.4
0.5
0.6
0.7
T /
−1
FIG. 11. Temperature dependence of χmax in the range β = 1.0, . . .
,6.0 eV−1. The lighter dots are from single lattices in the
infinite volume limit; the darker dots of matching colors are
obtained from average values of subsequent even and odd lattices.
The dotted lines are fits using Eq. (42) for χmax
con and Eq. (43) for χmax dis in
appropriate ranges (see text).
comparison of Figs. 10 (middle and bottom) it is clear that these
increases are driven mainly by the disconnected parts here, which
are once more unaffected by negative offsets from the Euclidean
time discretization, as observed in Sec. IV A already.
To detect deviations from the temperature-driven logarith- mic
divergence characteristic of the neck-disrupting Lifshitz
transition and described by Eq. (11), we simulate lattices with δ =
1/6 eV−1 in the range β = 1.0 . . . 6 eV−1 in steps of β = 0.5
eV−1. For these simulations, we focused on the immediate vicinity
of the VHS (the position of which does not depend strongly on
temperature), generating several points in a small interval around
it and using parabolic fits to identify the peak-positions and
heights of χ/χcon/χdis. Obtaining a proper infinite-size limit
becomes increasingly problematic for lower temperatures. In
particular for β = 5.0 eV−1 and larger, this turned out to be too
expensive to carry out in a brute-force way. Based on the
observation that the approach N → ∞ depends on the lattice parity,
i.e., whether its linear extend N is even or odd (see Fig. 4 and
the discussion thereof), we have thus devised a method to improve
convergence: Since even lattices overestimate the infinite-size
limit of χmax and odd lattices underestimate it, we may expect
faster convergence for average values of two subsequent lattices of
different parity. We have verified that this is indeed so with β =
4.0 and 4.5 eV−1, for which we compare the average values from the
N = 12 and 13 lattices with the converged large N results in Fig.
11. We then apply this averaging method for β = 5.0, 5.5, and 6
eV−1, where we have no brute-force results in the infinite-size
limit. We expect this method to break down close to a true
thermodynamic phase transition, as the usual finite-size scaling
relations would then apply, but for the β values up to 5.5
eV−1
successive average values from N = 11,12 and 11,12 lattices still
have converged with good accuracy.3
3The β = 6 eV−1 result still has somewhat reduced statistics
compared to the others, and it is likely to be affected by larger
systematic uncertainties from less control of finite-size
effects.
Figure 11 shows the temperature dependence of the result- ing
infinite-size estimates for the peak heights of χ/χcon/χdis
obtained in this way. We have identified a range of β = 1/T
between 1.0 and 3.0 eV−1 as the one over which a fit of the
form
f1(T ) = a ln
κ (41)
to the full susceptibility is possible (it breaks down if one
attempts to include lower temperatures). More interestingly,
however, the same fit to the connected part of the susceptibility
alone is consistent with a = 3/(π2κ) for β 2.5 eV−1 as pre- dicted
for the Lifshitz transition in the noninteracting system from Eq.
(11), despite the fact that we have simulated at full interaction
strength λ = 1 here. A two-parameter fit to the form
κ χmax con = 3
κ (42)
is included in Fig. 11, yielding b = 0.519(3) and, for the leading
O(T ) corrections in Eq. (11), c = −0.472(8) (a three- parameter
fit to the form in Eq. (41) produces κa = 0.307(32), i.e., a
central value in 1% agreement with κa=3/π2). The result for b is
furthermore quite close (within 13%) to the constant in Eq. (11) as
well, with a discrepancy that is within the expected offset from
the discretization δ = 1/6 eV−1
here. We may conclude that for the larger temperatures, where the
logarithmic scaling of the peak height is observed, the behavior of
the connected susceptibility basically fully agrees with that of
the noninteracting tight-binding model in Eq. (11).
At temperatures below T ∼ 0.15 κ this contribution from the
electronic Lifshitz transition, which we have successfully isolated
in χcon, suddenly drops in the interacting theory, however. This is
contrasted by a rapid increase of the peak height of the
disconnected susceptibility χdis here, which vanishes in the
noninteracting limit. While χdis is negligible at high
temperatures, it becomes the dominant contribution to the
susceptibility at T ∼ 0.07 κ . In fact, we find that for β 2.5 eV−1
(corresponding to T 0.15 κ), χmax
dis is well described by the model
f2(T ) = k
T − Tc
Tc
−γ
, (43)
resulting in the fit parameters listed in Table I. The emerging
peak in χmax
dis (T ) around β ≈ 6 eV−1 is thus consistent with a power-law
divergence indicative of a thermodynamic phase transition at
nonzero Tc. Despite our efforts to produce reliable estimates for
the infinite-size limits, we must expect, however, that there are
still residual finite-size effects in the points closest to Tc,
especially in the case of a continuous transition with a diverging
correlation length. Nevertheless, the case for a power-law
divergence at a finite temperature seems rather compelling here.
All attempts to model χmax
dis (T ) using a logarithmic increase as in Eq. (41)
TABLE I. Parameters resulting from a fit of Eq. (43) to χmax dis
(T).
βc[eV−1] Tc[κ] γ k[eV−1]
6.1(5) 0.060(5) 0.52(6) 0.12(1)
MICHAEL KÖRNER et al. PHYSICAL REVIEW B 96, 195408 (2017)
FIG. 12. χ sdw con (μ) (top) and χ sdw
dis (μ) (bottom) for β = 2 eV−1, N = 12 at different interaction
strengths. All displayed points are quadratic δ → 0 extrapolations
from simulations at nonzero δ.
were certainly unsuccessful, so that our conclusion seems
qualitatively robust and significant.
The two most important observations are as follows: (a) we observe
good evidence of a finite transition temperature Tc > 0 from the
behavior of the disconnected susceptibility as an indication of the
proximity to a thermodynamic phase transition as temperatures
approach this Tc ≈ 0.06 κ from above. (b) While the scaling
exponent γ ≈ 0.5 might also be interpreted as an indication of a
reshaping of the saddle points in the single-particle band
structure by the interelectron interactions according to Eq. (12)
with an exponent α ≈ 4 as discussed in Sec. II A,4 because of the
nonzero Tc it does not have this simple description in terms of
independent quasipar- ticles with modified single-particle
energies, however. Rather, it resembles critical behavior in the
vicinity of a second-order phase transition. This is in line with
our observation that here it arises in the disconnected
susceptibility as mentioned above.
D. Antiferromagnetic spin-density wave susceptibility
As explained in Sec. III A we have used here for purely
computational reasons a sublattice s and spin-staggered mass
4As such it would be at odds with the scenario of completely flat
bands (the large-α limit).
FIG. 13. Temperature dependence of χ sdw con (μ) (top) and χ
sdw
dis (μ) (bottom) for δ = 1/6 eV−1 and λ = 1. Lattice sizes scale
linearly with β, such that the displayed curves correspond to N =
12,18,24, respectively.
ms = (−1)s m in order to regulate the low-lying eigenvalues of the
fermion matrix near half filling. This has the effect of
introducing a small gap around the Dirac points in the single-
particle energy bands by triggering an antiferromagnetic order in
the ground state. For the interaction strengths 0 λ 1 considered
here, this order will disappear in the limit m → 0 because
suspended graphene with λ = 1 remains in the semimetal phase, which
has been established experimentally [82] as well as in our present
HMC simulation setup [51,53].
Nevertheless, we have also measured the corresponding
susceptibility χ sdw(μ) for the antiferromagnetic spin-density
fluctuations here. While we expect no singularity at half filling,
we were particularly interested in its behavior at finite μ in our
present study. With the same splitting into connected and
disconnected contributions, cf. Eqs. (40), our main observations
are the following: The systematics for discretization errors are
completely analogous to what was discussed above (a shift of the
connected part which is nearly independent of μ and almost no
effect on the disconnected part). As above, in Figs. 12 we again
first show the continuum extrapolated results at high temperature β
= 2 eV−1, where this is still affordable. We observe an increase of
χ sdw(μ = 0) at half filling with increasing interaction strength
as expected. However, in addition to this, a peak appears to form
at finite μ
for the larger values of λ, mainly in χ sdw con but to some
extend
195408-14
HYBRID MONTE CARLO STUDY OF MONOLAYER . . . PHYSICAL REVIEW B 96,
195408 (2017)
also visible in χ sdw dis which again vanishes in the
noninteracting
system, of course. This peak occurs about halfway between μ = 0 and
the
VHS in the vicinity of μ = κ . When the temperature is lowered,
however, it it appears to move toward the VHS while getting more
pronounced. This is demonstrated with the ensembles at finite
discretization δ = 1/6 eV−1 but lower tem- peratures and maximal
interaction strength λ = 1 in Figs. 13. As before, there is no
negative offset from the Euclidean-time discretization in the
disconnected susceptibility which shows the increasingly sharp peak
structure at the lower temperatures particularly well. Whether the
peaks observed in the discon- nected susceptibilities of
ferromagnetic and antiferromagnetic spin-density fluctuations
eventually merge and perhaps reflect the same thermodynamic phase
transition when approaching Tc certainly deserves to be further
studied in the future.
V. SUMMARY AND CONCLUSIONS
We have set out to study the effects of interelectron interactions
on the electronic Lifshitz transition in graphene. This
neck-disrupting Lifshitz transition occurs when the Fermi level
traverses the van Hove singularity at the M points in the band
structure of graphene. To elucidate the effects of interactions, we
have first discussed in detail how the Lifshitz transition is
reflected in the particle-hole susceptibility of the noninteracting
system, where it is due to a logarithmic singularity of the density
of states. In particular, we have demonstrated how this singularity
translates into a logarithmic growth of the susceptibility maximum,
when viewed as a func- tion of the chemical potential, with
decreasing temperature and increasing system size.
The detailed analytical knowledge of the behavior of the
particle-hole susceptibility in the noninteracting system, where it
agrees with the ferromagnetic spin susceptibility, allowed us to
isolate the same Lifshitz behavior also in presence of strong
interelectron interactions, where it would otherwise have swamped
any signs of thermodynamic singularities indicative of true phase
transitions.
To search for such signs, we have simulated the π -band electrons
in monolayer with partially screened Coulomb interactions,
combining realistic short-distance couplings with long-range
Coulomb tails, using Hybrid Monte Carlo. This requires a chemical
potential with a spin-dependent sign to circumvent the fermion-sign
problem, however. We were therefore led to compare the
ferromagnetic spin suscepti- bility with that of the noninteracting
system. Despite this modification, our results qualitatively
resemble some of the experimental results at finite charge-carrier
density. An increase of its peak height due to interactions is in
line with the existence of an extended van Hove singularity (EVHS)
as observed in ARPES experiments [10]. Likewise, we observe band
structure renormalization (narrowing of the widths of the π bands)
due to interactions and doping [31] here as well. An interesting
feature of our results is a second peak in the spin susceptibility
χ (μ) which arises near the upper end of the band. Whether this is
due to some form of condensation of quasiparticle pairs near the
points, which might happen because the Fermi levels of the
different spin components were shifted in opposite directions,
remains to be further studied.
The electronic Lifshitz transition itself is reflected in the
connected part of the susceptibility χcon(μ) which diverges
logarithmically in the T → 0 limit when μ is at the van Hove
singularity. In the noninteracting system, χ (μ) = χcon(μ) and
χdis(μ) = 0. With interactions, on the other hand, one has χ (μ) =
χcon(μ) + χdis(μ). Interestingly, however, for higher temperatures
where χdis(μ) is comparatively small, the behavior of χcon(μ)
remains precisely the same as in the noninteracting case. The
electronic Lifshitz transition is entirely encoded in χcon(μ). Upon
its subtraction from the full susceptibility, one is left with
χdis(μ), which is moreover expected to be the relevant part in
search for a thermodynamic singularity, reflecting a phase
transition.
In fact, our simulations provide evidence of such a thermodynamic
singularity. Our results are consistent with a power-law divergence
of χdis at an electron temperature of about Tc ≈ 0.16 eV ≈ 0.06 κ ,
which suggests that the Lifshitz transition is replaced in the
interacting theory by a true quantum phase transition below Tc, and
hence for T → 0, with μ as the control parameter. Without
identifying and isolating the Lifshitz behavior in χcon(μ), it
would not have been possible to observe this with our present
computational resources (we have already invested several hundreds
of thousands of GPU hours in this project). The thermodynamic
singularity is basically not visible in our present data for the
full susceptibility although it will eventually dominate,
sufficiently close to Tc, of course.
There are a number of possible directions for future work on the
VHS. The most straightforward albeit expensive extension would be
an analysis of the critical scaling close to Tc. Furthermore, of
direct practical interest would be a comparison of susceptibilities
associated with different types of ordered phases such as that of
the antiferromagnetic spin-density wave order parameter studied as
a first example at the end of the last section, or superconducting
phases (e.g., chiral superconductivity [13]). It should in
principle be possible to identify the dominant instability of the
VHS and a corresponding pairing channel.
Since the relevance of electron-phonon couplings at the VHS was
demonstrated experimentally [24], a quantitatively exact result
should only be expected when phonons are accounted for.
Furthermore, as was demonstrated, e.g., in Ref. [14], deviations
from exact Fermi-surface nesting have a profound impact on the
competition between ordered phases. This implies that for a
realistic description the inclusion of higher order hoppings, which
suffer from a fermion-sign problem, will be necessary. For this
reason, and due to the obvious fact that finite spin and
charge-carrier densities have different ground states, there is a
solid motivation for efforts toward dealing with the sign problem.
As the Hubbard field introduced in this work has a much simpler
structure than a non-Abelian gauge theory, it is conceivable that
some of the more recent developments [64,67,73,74] mentioned in
Sec. III B will turn out to be useful in this context.
ACKNOWLEDGMENTS
This work was supported by the Deutsche Forschungsge- meinschaft
(DFG) under Grants No. BU 2626/2-1 and No.
195408-15
MICHAEL KÖRNER et al. PHYSICAL REVIEW B 96, 195408 (2017)
SM 70/3-1. Calculations have been performed on GPU clusters at the
Universities of Giessen and Regensburg. P.B. is also
supported by a Sofia Kowalevskaja Award from the Alexander von
Humboldt foundation.
[1] P. R. Wallace, Phys. Rev. 71, 622 (1947). [2] V. P. Gusynin, S.
G. Sharapov, and J. P. Carbotte, Int. J. Mod.
Phys. B 21, 4611 (2007). [3] I. Lifshitz, Sov. Phys. JETP 11, 1130
(1960). [4] L. van Hove, Phys. Rev. 89, 1189 (1953). [5] B. Dietz,
F. Iachello, M. Miski-Oglu, N. Pietralla, A. Richter,
L. von Smekal, and J. Wambach, Phys. Rev. B 88, 104101
(2013).
[6] B. Dietz, T. Klaus, M. Miski-Oglu, A. Richter, M. Wunderle, and
C. Bouazza, Phys. Rev. Lett. 116, 023901 (2016).
[7] B. Dietz, T. Klaus, M. Miski-Oglu, A. Richter, M. Bischoff, L.
von Smekal, and J. Wambach, Phys. Rev. Lett. 115, 026801
(2015).
[8] W. Kohn and J. M. Luttinger, Phys. Rev. Lett. 15, 524 (1965).
[9] R. S. Markiewicz, J. Phys. Chem. Solids 58, 1179 (1997).
[10] J. L. McChesney, A. Bostwick, T. Ohta, T. Seyller, K. Horn, J.
González, and E. Rotenberg, Phys. Rev. Lett. 104, 136803
(2010).
[11] W. S. Wang, Y. Y. Xiang, Q. H. Wang, F. Wang, F. Yang, and D.
H. Lee, Phys. Rev. B. 85, 035414 (2012).
[12] J. González, Phys. Rev. B 78, 205431 (2008). [13] R.
Nandkishore, L. S. Levitov, and A. V. Chubukov, Nat. Phys.
8, 158 (2012). [14] M. L. Kiesel, C. Platt, W. Hanke, D. A. Abanin,
and R. Thomale,
Phys. Rev. B 86, 020507 (2012). [15] M. Yu. Kagan, V. V. Val’kov,
V. A. Mitskan, and M. M.
Korovushkin, Solid State Commun. 188, 61 (2014). [16] A. M.
Black-Schaffer and C. Honerkamp, J. Phys.: Condens.
Matter 26, 423201 (2014). [17] T. Löthman and A. M. Black-Schaffer,
Phys. Rev. B 90, 224504
(2014). [18] J. González, Phys. Rev. B 88, 125434 (2013). [19] D.
Makogon, R. van Gelderen, R. Roldán, and C. M. Smith,
Phys. Rev. B 84, 125404 (2011). [20] B. Valenzuela and M. A. H.
Vozmediano, New J. Phys. 10,
113009 (2008). [21] C. A. Lamas, D. C. Cabra, and N. Grandi, Phys.
Rev. B 80,
075108 (2009). [22] J. P. L. Faye, M. N. Diarra, and D. Sénéchal,
Phys. Rev. B 93,
155149 (2016). [23] M. Cranney, F. Vonau, P. B. Pillai, E. Denys,
D. Aubel, M. M.
D. Souza, C. Bena, and L. Simon, Europhys. Lett. 91, 66004
(2010).
[24] J. L. McChesney, A. Bostwick, T. Ohta, K. V. Emtsev, T.
Seyller, K. Horn, and E. Rotenberg, arXiv:0705.3264.
[25] K. S. Novoselov, A. K. Geim, S. V. Morozov, D. Jiang, M. I.
Katsnelson, I. V. Grigorieva, S. V. Dubonos, and A. A. Firsov,
Nature (London) 438, 197 (2005).
[26] Y. Zhang, Y. W. Tan, H. L. Stormer, and P. Kim, Nature
(London) 438, 201 (2005).
[27] D. K. Efetov and K. Philip, Phys. Rev. Lett. 105, 256805
(2010).
[28] G. Li, A. Luican, J. M. B. Lopes dos Santos, A. H. Castro
Neto, A. Reina, J. Kong, and E. Y. Andrei, Nat. Phys. 6, 109
(2010).
[29] A. Bostwick, T. Ohta, J. L. McChesney, T. Seyller, K. Horn,
and E. Rotenber, Solid State Commun. 143, 63 (2007).
[30] V. Y. Irkhin, A. A. Katanin, and M. I. Katsnelson, Phys. Rev.
Lett. 89, 076401 (2002).
[31] S. Ulstrup, M. Schüler, M. Bianchi, F. Fromm, C. Raidel, T.
Seyller, T. Wehling, and P. Hofmann, Phys. Rev. B 94, 081403
(2016).
[32] I. L. Aleiner, D. E. Kharzeev, and A. M. Tsvelik, Phys. Rev. B
76, 195415 (2007).
[33] T. O. Wehling, E. Sasioglu, C. Friedrich, A. I. Lichtenstein,
M. I. Katsnelson, and S. Blugel, Phys. Rev. Lett. 106, 236805
(2011).
[34] T. Stauber, Phys. Rev. B 82, 201404(R) (2010). [35] J. P.
Hobson and W. A. Nierenberg, Phys. Rev. 89, 662 (1953). [36] A. H.
Castro Neto et al., Rev. Mod. Phys. 81, 109 (2009). [37] Y. M.
Blanter, A. V. Pantsulaya, and A. A. Varlamov, Phys. Rep.
245, 159 (1994). [38] R. Brower, C. Rebbi, and D. Schaich, PoS
LATTICE 2011, 056
(2012). [39] R. Brower, C. Rebbi, and D. Schaich, arXiv:1101.5131.
[40] J. E. Drut and T. A. Lähde, Phys. Rev. Lett. 102, 026802
(2009). [41] J. E. Drut and T. A. Lähde, Phys. Rev. B 79, 165425
(2009). [42] J. E. Drut and T. A. Lähde, Phys. Rev. B 79, 241405
(2009). [43] J. E. Drut, T. A. Lähde, and L. Suoranta,
arXiv:1002.1273. [44] J. E. Drut and T. A. Lähde, PoS LATTICE 2011,
074 (2011). [45] S. Hands and C. Strouthos, Phys. Rev. B 78, 165423
(2008). [46] W. Armour, S. Hands, and C. Strouthos, Phys. Rev. B
81, 125105
(2010). [47] W. Armour, S. Hands, and C. Strouthos, Phys. Rev. B
84, 075123
(2011). [48] P. V. Buividovich, E. V. Luschevskaya, O. V.
Pavlovsky, M.
I. Polikarpov, and M. V. Ulybyshev, Phys. Rev. B 86, 045107
(2012).
[49] J. Giedt, A. Skinner, and S. Nayak, Phys. Rev. B 83, 045420
(2011).
[50] P. V. Buividovich and M. I. Polikarpov, Phys. Rev. B 86,
245117 (2012).
[51] M. V. Ulybyshev, P. V. Buividovich, M. I. Katsnelson, and M.
I. Polikarpov, Phys. Rev. Lett. 111, 056801 (2013).
[52] D. Smith and L. von Smekal, PoS LATTICE 2013, 048 (2013). [53]
D. Smith and L. von Smekal, Phys. Rev. B 89, 195429 (2014). [54] D.
Smith, M. Körner, and L. von Smekal, PoS LATTICE 2014,
055 (2014). [55] P. Buividovich, D. Smith, M. Ulybyshev, and L. von
Smekal,
PoS LATTICE 2016, 244 (2016). [56] D. L. Boyda, V. V. Braguta, M.
I. Katsnelson, and M. V.
Ulybyshev, Phys. Rev. B 94, 085421 (2016). [57] M. V. Ulybyshev and
M. I. Katsnelson, Phys. Rev. Lett. 114,
246801 (2015). [58] P. Buividovich, D. Smith, M. Ulybyshev, and L.
von Smekal,
Phys. Rev. B 96, 165411 (2017). [59] T. Luu and T. A. Lähde, Phys.
Rev. B 93,155106 (2016). [60] H. K. Tang, E. Laksono, J. N. B.
Rodrigues, P. Sengupta,
F. F. Assaad, and S. Adam, Phys. Rev. Lett. 115, 186602
(2015).
HYBRID MONTE CARLO STUDY OF MONOLAYER . . . PHYSICAL REVIEW B 96,
195408 (2017)
[61] S. Raghu, X.-L. Qi, C. Honerkamp, and S.-C. Zhang, Phys. Rev.
Lett. 100, 156401 (2008).
[62] S. Duane, A. D. Kennedy, B. J. Pendleton, and D. Roweth, Phys.
Lett. B 195, 216 (1987).
[63] K. Langfeld, B. Lucini, and A. Rago, Phys. Rev. Lett. 109,
111601 (2012).
[64] K. Langfeld and B. Lucini, Phys. Rev. D 90, 094502 (2014).
[65] N. Garron and K. Langfeld, Eur. Phys. J. C 76, 569 (2016).
[66] S. Chandrasekharan and U. J. Wiese, Phys. Rev. Lett. 83,
3116
(1999). [67] E. F. Huffman and S. Chandrasekharan, Phys. Rev. B 89,
111101
(2014). [68] Z.-X. Li, Y.-F. Jiang, and H. Yao, Phys. Rev. B 91,
241117(R)
(2015). [69] Z. C. Wei, C. Wu, Y. Li, S. Zhang, and T. Xiang, Phys.
Rev. Lett.
116, 250601 (2016). [70] Z.-X. Li, Y.-F. Jiang, and H. Yao, Phys.
Rev. Lett. 117, 267002
(2016). [71] N. Prokof’ev and B. Svistunov, Phys. Rev. Lett. 87,
160601
(2001).
[72] Y. Delgado Mercado, C. Gattringer, and A. Schmidt, Phys. Rev.
Lett. 111, 141601 (2013).
[73] A. Mukherjee and M. Cristoforetti, Phys. Rev. B 90, 035134
(2014).
[74] A. Alexandru, G. Basar, P. F. Bedaque, G. W. Ridgway, and N.
C. Warrington, Phys. Rev. D 95, 014502 (2017).
[75] D. Sexty, PoS LATTICE 2014, 016 (2014). [76] T. Boz, P.
Giudice, S. Hands, J. I. Skullerud, and A. G. Williams,
AIP Conf. Proc. 1701, 060019 (2016). [77] L. Holicki, J. Wilhelm,
D. Smith, B. Wellegehausen, and L. von
Smekal, PoS LATTICE 2016, 052 (2017). [78] A. Maas, L. von Smekal,
B. Wellegehausen, and A. Wipf,
Phys. Rev. D 86, 111901 (2012). [79] B. H. Wellegehausen and L. von
Smekal, PoS LATTICE 2014,
177 (2015). [80] W. Detmold, K. Orginos, and Z. Shi, Phys. Rev. D
86, 054507
(2012). [81] B. B. Brandt and G. Endrodi, PoS LATTICE 2016,
039
(2016). [82] D. C. Elias et al., Nat. Phys. 7, 701 (2011).
LOAD MORE